- Research Article
- Open Access
Adsorption of copper (II) on mesoporous silica: the effect of nano-scale confinement
© National Technology of Engineering Solutions of Sandia, LLC 2018
Received: 26 February 2018
Accepted: 8 June 2018
Published: 26 June 2018
Nano-scale spatial confinement can alter chemistry at mineral–water interfaces. These nano-scale confinement effects can lead to anomalous fate and transport behavior of aqueous metal species. When a fluid resides in a nanoporous environments (pore size under 100 nm), the observed density, surface tension, and dielectric constant diverge from those measured in the bulk. To evaluate the impact of nano-scale confinement on the adsorption of copper (Cu2+), we performed batch adsorption studies using mesoporous silica. Mesoporous silica with the narrow distribution of pore diameters (SBA-15; 8, 6, and 4 nm pore diameters) was chosen since the silanol functional groups are typical to surface environments. Batch adsorption isotherms were fit with adsorption models (Langmuir, Freundlich, and Dubinin–Radushkevich) and adsorption kinetic data were fit to a pseudo-first-order reaction model. We found that with decreasing pore size, the maximum surface area-normalized uptake of Cu2+ increased. The pseudo-first-order kinetic model demonstrates that the adsorption is faster as the pore size decreases from 8 to 4 nm. We attribute these effects to the deviations in fundamental water properties as pore diameter decreases. In particular, these effects are most notable in SBA-15 with a 4-nm pore where the changes in water properties may be responsible for the enhanced Cu mobility, and therefore, faster Cu adsorption kinetics.
Developing a better understanding of the chemistry at mineral surfaces is critical to predict the fate and transport of chemical species in soils, sediments, and in porous rocks . Interfacial processes, taking place at the atomic scale: ~ 10−10 m can manifest all the way to the scale of planet Earth: ~ 107 m, and the chemistry at surfaces depend on the spatial environment of the surface . Nano-scale confined domains are ubiquitous in the environment and exist in tight rocks (i.e. shale), where large fraction of pores are in the nano-scale range [2, 3]. These domains have been recognized as an important factor in the selective permeability of tight rocks, a phenomenon largely attributed to the compressed electrical double layer at the water–solid interface as the pores decrease in size . These nano-scale domains can be defined as microporous (< 2 nm pore diameter), mesoporous (2–50 nm pore diameter), and macroporous (> 50 nm pore diameter) [4, 5]. When fluids reside in these nano-pores, the observed thermodynamic properties of these systems deviate from those measured in bulk non-confined phases . Previous research has shown, that with decreasing pore size, the fundamental properties of water change, which is expected to affect the adsorption of ions at mineral–water interfaces. Examples of these deviations in water properties include a decrease in the dielectric constant (as much as a 50% decrease with a 1.2 nm pore) [7, 8], density, and surface tension when the pore size is less than 5 nm . These deviations are largely attributed to the high ratio of mineral-surface-bound (structured) water in nano-scale confined systems relative to bulk water .
Stimulated by the advances in the nanotechnology industry, nanogeochemistry has emerged as an active field of research and has led to numerous observations of size-dependent phenomena, including metal adsorption on mineral surfaces . Propagated from changes in water properties, an observed decrease in the solvation energies and an increase in the formation of inner-sphere complexes of metal cations can lead to enhanced adsorption [2, 10, 11]. Research has demonstrated these effects, showing an enhanced adsorption of arsenic (As) on ordered mesoporous alumina compared to non-porous activated alumina , and enhanced copper (Cu) and uranium (U) adsorption with decreasing hematite particle size [13, 14]. Furthermore, the adsorption mode for various adsorbed metals on zeolites with nanopores changed from outer sphere to inner sphere as the pore became smaller [15–17]. The adsorption of Cu on zeolites with narrow pores (0.26–0.74 nm) has been investigated with electron paramagnetic resonance spectroscopy and demonstrated an enhanced adsorption and increased inner sphere coordination in the zeolites with the smallest pores . While these studies have illustrated the deviation in thermodynamic properties when mineral particles are limited to nano-scale, using natural mineral surfaces (i.e. hematite) or compared porous versus non-porous material, there has yet to be a study that takes a systematic approach to evaluate the adsorption properties of metal cations as a function of discrete incremental changes in the pore size.
In this study, the adsorption of Cu2+ was evaluated on mesoporous silica. Copper was chosen as an analyte because it is an important naturally-occurring trace element with abundance in the Earth’s crust of 50 mg kg−1 . Copper is mined for its wide use in industrial applications, and as a result, can reach toxic concentrations in environmental systems [18–22]. At trace concentrations, Cu is essential for life, and is involved in many enzymatic reactions in mammals . Industrially, Cu has applications in the electrical industry, in the production of alloys, as a catalysis, and much more [18, 19]. As a result, the total anthropogenic discharge ranges from 35,000 to 90,000 metric tons per year . Therefore, Cu is a common environmental pollutant where most of the Cu release is resulting from acid mine drainage and landfill leachates . Understanding the adsorption properties of Cu and how the adsorption properties are impacted by nano-scale confinement is important in broadening our understanding of the fate and transport of Cu in a variety of complex environmental and geological systems. Additionally, using Cu2+ to probe the reactivity of confined interfaces, allowed us to quantify size-dependent behavior. Previous research has investigated the adsorption of Cu2+ on functionalized ordered mesoporous silica and alumina to assess Cu2+ removal for water treatment purposes [21–23]. Adsorption was significantly enhanced by the addition of functional groups N-[3-(trimethoxysilyl)propyl]-ethylenediamine, from 0.036 mmol Cu g−1 on unmodified silica to 0.261 mmol Cu g−1 on functionalized silica . Modifying the silica substrate allowed for significant removal of Cu2+ from aqueous solution, but in doing so, the pore geometry, volume, and reactivity were altered; and no longer represented an environmentally equivalent (e.g. silicate) system. To evaluate the effects of nano-scale confinement with environmentally relevant reactive surfaces, we focused on unmodified mesoporous silica to present the first study, to our knowledge, that directly investigated the impact of pore size on the Cu2+ adsorption kinetics and uptake.
Ordered mesoporous silica is an ideal candidate to assess the impacts of nano-scale confinement on the adsorption of Cu2+. These materials are synthetically produced via a surfactant template, creating chemically stable high surface area structures with uniform pores and a narrow distribution of pore diameters . These synthetic mesoporous materials are representative of the reactive surface sites typical on mineral surfaces, containing silanol functional groups (i.e. silicates) . For our investigations, we utilized three analogues mesoporous silica substrates (SBA-15) with different size pore diameters, 8 nm (SBA-15-8), 6 nm (SBA-15-6), and 4 nm (SBA-15-4) diameter, all having cylindrical pore geometry. These SBA-15 siliceous materials are produced by templating triblock copolymers to create a two-dimensional hexagonal array of non-intersecting cylindrical pores [25, 26]. This range of pore diameters (8, 6, and 4 nm) represents the scale at which nano-scale confinement effects have been determined to be most significant [8, 9]. We hypothesized that the adsorption of Cu2+ on mesoporous silica is pore size dependent, and suspect, as pore size decrease and confined water properties emerge, Cu2+ adsorption will be enhanced.
The goal of this study was to systematically assess the surface complexation of Cu2+ under nano-scale confinement in model mesoporous materials using batch adsorption isotherms and kinetics studies. The adsorption isotherms were fit to adsorption isotherm models (Langmuir, Freundlich, and Dubinin–Radushkevich) to extract adsorption parameters, and pseudo-first-order kinetics model to extract rate constants. This data was used to evaluate the impact of nano-scale confinement on the surface area normalized adsorptive behavior of Cu2+ on mesoporous silica.
All reagents used for batch adsorption studies were reagent grade or higher, including copper(II) nitrate trihydrate (Cu(NO3)2·3H2O), ammonium nitrate (NH4NO3), nitric acid (HNO3), and ammonium hydroxide (NH4OH) (Sigma-Aldrich, St. Louis, MO). Ultrapure HNO3 (ULTREX II, J. T. Baker, Thermo Fisher Scientific, Waltham, MA) was used for dilutions and sample preservation. Aqueous concentrations of Cu2+ were quantified via inductively coupled plasma mass spectrometer (ICP-MS) (NexION 350D, Perkin Elmer, Waltham, MA). All gasses and cryogenic liquids used for ICP-MS analysis and Brunauer–Emmett–Teller (BET) surface area analysis were ultrapure quality grade (Matheson, Basking Ridge, NJ) including liquid and gaseous argon (Ar) and nitrogen (N2), along with helium (He) gas. All mesoporous materials were purchased from Sigma Aldrich (Sigma Aldrich, St. Louis, MO). These materials included SBA-15-8, SBA-15-6, SBA-16-4 correspond to hexagonally ordered cylindrical pores with diameters of 4, 6, and 8 nm. Milli-Q H2O (Barnstead NANOpure Diamond, resistivity of 18.2 MΩ*cm, 0.2 μm filtered and UV irradiated) was used in the preparation of all solutions and suspensions.
BET surface area and pore size determination
The BET surface area for each mesoporous material was obtained using two different BET surface area analyzers, an ASAP 2020 (Micrometrics, Norcross, GA) and a TriStar (Micrometrics, Norcross, GA). The procedure on both instruments was the same. Approximately 200 mg of dry mesoporous material was transferred into a tarred BET tube equipped with an airtight cap. The samples were degassed at 300 °C for 4 h and backfilled with inert He gas. Following the sample degas, the mass of the sample was updated to account for mass changes in the resulting from the degas. Next, the liquid N2 Dewar was filled, a thermal jacket was placed on the BET tube, the tube was placed in the sample holder, and the analysis was started. The surface area analyzer determined the BET surface area and the non-local density functional theory (NLDFT) method was used to determine pore diameter and volume for each SBA-15 substrate [26, 27].
Thermogravimetric analysis (TGA; Thermal Analysis, SDT Q600, New Castle, DE) was performed on SBA-15-4, SBA-15-6, and SBA-15-8 to estimate the hydroxyl group density. Prior to analysis each silica material was thoroughly rinsed and dried. Briefly, approximately 600 mg of mesoporous material was added to centrifuge bottle with 200 mL of Milli-Q water and mixed on a shaker table (Orbital-Genie, Scientific Industries, INC, Bohemia, New York). Following shaking for 24 h the materials were filtered (45 μm, Pall Corporation, Ann Arbor, MI), and rinsed with Milli-Q water and suspended in 200 mL of Milli-Q water. This process was repeated two additional times. Following the final rinse, the mesoporous materials were transferred to a scintillation vial and placed in the oven (45 °C) for at least 48 h. Once dry, roughly 10 mg silica was transferred to a tarred TGA crucible (100 μL, Robocasting, Albuquerque, NM) and placed in the TGA furnace. The flow rate of Ar was 100 mL/min with an experimental sequence: (i) 20 min room temperature isothermal to equilibrate, (ii) ramp temperature at 10 °C/min from room temperature to 1000 °C.
Batch adsorption and adsorption isotherms
Batch adsorption isotherm experiments were performed to evaluate the adsorption of Cu2+ on SBA-15-8, SBA-15-6, and SBA-15-4. The SBA-15 materials were rinsed prior to use, as described above (same method as TGA). Following being rinsed and dried, approximately 20 mg was weighed out and transferred to a 50 mL centrifuge tube with 5 mL of 10 mM NH4NO3 and rehydrated for at least 24 h. The electrolyte, NH4NO3, was chosen as the background electrolyte to prevent adding any metal cationic species to compete for surface adsorption sites. Following 24 h, Cu(NO3)2 was added to each 50 mL centrifuge tube with a concentration of Cu2+ ranging from 5 to 300 μM from a stock Cu(NO3)2 solution and brought up to 10 mL total volume with Milli-Q water. The pH was adjusted using dilute solutions of HNO3 and NH4OH to achieve a final pH of 6.0 ± 0.1 and final ionic strength of 10 ± 1 mM. Under these experimental conditions the dominant aqueous Cu species is Cu2+ (roughly 96%, estimated using Visual MINTEQ 3.1) . A detailed Cu speciation diagram is provided in Additional file 1: Figure S1. The contents were mixed via shaker table for 24 h. After mixing, the samples were centrifuged (Allegra 25R, Beckman Coulter, Indianapolis, IN) at 3000 rpm for 10 min to separate the solid mesoporous silica from the supernatant electrolyte solution. To fully separate the phases and remove any suspended mesoporous silica, the supernatant was transferred to a 10 mL syringe fit with a 0.20 μm nylon filter (Millex-GN, EMD Millipore, Billerica, MA) and the contents pushed through to a 15 mL centrifuge tube. Ultra pure 6 M HNO3 was added to each sample (10 μL mL−1) for sample preservation to keep Cu2+ cations from hydrolyzing and precipitating.
The samples were diluted to a concentration range suitable for Cu quantification via ICP-MS (10–2000 ppb). Dilutions were performed using Ultrapure 2% HNO3 by a factor of 2, 5, 10, or 50 and kept in the refrigerator until the ICP-MS analysis. The experimental data was fit to three adsorption isotherm models: Langmuir, Freundlich, and Dubinin–Radushkevich.
Langmuir adsorption isotherm
The equilibrium parameter provides an understanding of the favorability of the adsorption as a function of the initial concentration of adsorbate, when RL > 1 the adsorption is unfavorable, 0 < RL < 1 the adsorption is favorable, and when R = 0 the adsorption is irreversible [30, 34].
Freundlich adsorption isotherm
It should be noted that the Freundlich isotherm does not accurately determine the absolute maximum adsorbed Cu . This is due to the fact that qe is directly proportional to [Cu2+]eq, and therefore qe will increase as [Cu2+]eq increases. Yet, the KF value can be used as a qualitative comparison to assess the relative adsorption maximum values of Cu on mesoporous silica surfaces.
Dubinin–Radushkevich adsorption isotherm
The fitting parameters qm−DR and kDR are determined by the intercept and slope, respectively, of a the linear line when plotted ln (qe) versus ε2.
Kinetic studies were performed to determine the rate law of the Cu adsorption on mesoporous materials, and to quantify the effect of nano-scale confinement on the adsorption rates. For these studies, 100 mg of hydrated mesoporous silica was transferred to a 100 mL beaker with 25 mL of 10 mM NH4NO3, a stir bar set to vigorously mix the solution at 300 rpm and enough DI water to achieve a final volume of 50 mL. The solution pH was adjusted using HNO3 and NH4OH to a pH = 6.0 ± 0.1. Following the pH adjustment, a known amount of Cu2+ was spiked into the solution (5–10 μM Cu). The time and pH were recorded at this point and represented time = 0. The pH was continuously monitored by the pH probe as 3 mL aliquots were removed at set time points during the experiment and transferred to a 10 mL syringe and filtered into a 15 mL centrifuge tube containing 30 μL ultra pure 6 M HNO3. The kinetic studies ran for 6 h to establish an equilibrium value for adsorbed Cu (qe). This procedure was repeated at three concentrations of Cu2+ for each silica material.
Following the kinetic experiments, the samples representing unique time points (minutes) were diluted by a factor of 3 with Ultrapure 2% HNO3 for Cu quantification by ICP-MS. The diluted samples were kept in the refrigerator until sample analysis for Cu.
Pseudo-first-order adsorption kinetics
Batch kinetic adsorption studies were performed and fit to a pseudo-first-order reaction model. The rate constants for the adsorption of Cu on SBA-15-4, SBA-15-6, and SBA-15-8 were determined from the model fit. The pseudo-first-order reactions occur when the reaction is second order, however, one of the reactants is in excess and largely remains unchanged . In this case, three different dilute initial Cu2+ concentrations were reacted with 100 mg of mesoporous material. This is consistent with the fact that we had low Cu2+ concentrations and high silica reactive surface area.
Results and discussion
From studies investigating Cu adsorption on SBA-15-8, SBA-15-6, and SBA-15-4, we systemically evaluated the effects of nano-scale confinement. The sum of these effects provide insight into how nano-scale confinement can enhance metal adsorption in meso- and nano-porous materials.
BET surface area and pore size distribution
Pore size and BET surface area of SBA-15-8, SBA-15-6, and SBA-15-4
Pore size (nm)
BET surface area (m2/g)
Pore volume (cm3/g)
% surface area from pores
7.0 ± 0.3
661 ± 5
1.21 ± 0.03
89 ± 6
1.8 ± 0.2
5.2 ± 0.2
603 ± 16
0.87 ± 0.03
80 ± 5
1.9 ± 0.2
4.4 ± 0.1
580 ± 13
0.67 ± 0.04
75 ± 6
2.3 ± 0.2
The pore diameters were determined using the NLDFT method [26, 27]. The pore size distribution plots are shown in Additional file 1: Figure S2. The mesopore diameter is relatively narrow distribution resulting in average pore diameters and volumes reported in Table 1. As reported in previous pore size distributions of SBA-15 materials, there are micropores present as well [26, 41, 42]. The mesopores exist in the main channels as templated from the removal of the calcined surfactant, whereas the micropores co-exist due to intrawall pores that develop as a consequence of the removal of the surfactant template creating structural irregularities . This can be seen in the SBA-15-4 plot (Additional file 1: Figure S2), in which the pore size distribution is bimodal with peaks centered around 4.4 and 2 nm. In contrast, the SBA-15-8 (Additional file 1: Figure S2) shows a primary contribution from the mesopores centered around 8 nm, and a small contribution of micropores centered around 2 nm. For this study, we considered the average pore size diameter to assess the effects of nano-scale confinement. While the observed effects may be attributed to the increased presence of micropores, the micropores are defined by one data point and we believe appropriate nano-scale confinement conclusions can be drawn from adsorption deviations of Cu with these substrates.
Cu adsorption isotherms and nano-scale confinement effects
Fitting parameters obtained from the linear transformation of the data for Langmuir, Freundlich, and Dubinin–Radushkevich adsorption models
2.0 ± 0.4
0.057 ± 0.008
1.23 ± 0.03
0.060 ± 0.002
3.4 × 10−8 ± 8 × 10−9
0.0251 ± 0.001
2.7 ± 0.6
0.05 ± 0.01
1.36 ± 0.08
0.053 ± 0.004
3.0 × 10−8 ± 8 × 10−9
0.024 ± 0.002
3.6 ± 0.6
0.10 ± 0.01
1.27 ± 0.06
0.17 ± 0.01
2.9 × 10−8 ± 8 × 10−9
0.0622 ± 0.002
An assessment of the qualitative adsorption parameters (KL, n, and KD–R) shows that the adsorption affinities are generally similar for all three silica materials [29, 35, 37]. The qualitative adsorption parameter KL and KD–R (KD–R term in inversely proportional to adsorption affinity) suggest the adsorption affinity in the Langmuir and Dubinin–Radushkevich isotherm models are pore size dependent, while n has no pore size dependency trend as shown in Table 2. These terms qualitatively describe the adsorption affinity, suggesting there may be an increased adsorption affinity of Cu as the pore size decreases.
Additional information can be gleaned from the values of KL. From the KL value, RL can be approximated from Eq. 3. A plot of RL versus [Cu]initial (Additional file 1: Figure S3) estimates the reaction coordinate based upon differences in the KL values. The values of RL decrease with increasing Cu2+ concentration and remain between 1 and 0. This shows, as Cu2+ increases in the system, surface sites become occupied, thus the surface reaction decreases, but remains favorable. It was also found that the KL for SBA-15-4 pore was the lowest, indicating the most rapid decay of the RL term as a function of [Cu]initial. At the maximum [Cu]initial = 0.3 mM, the RL values are 0.63, 0.55 and 0.48 for SBA-15-8, SBA-15-6, and SBA-15-4, respectively. At the maximum adsorbed values of Cu, only 1% of the total –OH groups were occupied. The reactive surface sites are in excess compared to Cu and therefore the reaction favors the formation of surface complexes. Because these values are between 1 and 0, the surface adsorption reaction is still favorable; which suggests either, (i) the monolayer surface coverage has not reached a maximum value, or (ii) that multi-layer adsorption (i.e. dimerization, polymerization, or precipitation) occurs even at low surface coverages.
Additional work is planned to assess the coordination chemistry of Cu as a function of pore size to determine whether mechanistic changes result from nano-scale confinement. The current reaction condition, pH = 6, is above the point of zero charge, pzc, of SBA-15 silica (pzc = 4.2) . As a result, the silica surface is expected to be negatively charged, and the electrostatic interactions could be driving forces leading to the adsorption of free Cu2+ cations onto the silica surface. Building off the X-ray absorption data analysis by Cheah et al., Cu forms inner-sphere surface complexes with amorphous silica [19, 20]. Additional analyses observed short Cu–Cu distances (2.58–2.59 Å), suggesting the formation of dimeric species adsorbed onto the amorphous silica surface. The bonding mode was concluded to be mono-dentate, demonstrated from the presence of only one unique Cu–Si distance (~ 3.0 Å), whereas a bidentate-bridging bonding mode would have resulted in two unique Cu–Si distances, distinguishable spectroscopically [19, 20]. However, with decreasing pore size, to a pore regime where nano-scale confinement effects may become apparent, it is unclear if the adsorption mode and Cu adsorption complex geometry would remain constant. Ferreira et al. demonstrated that Cu contains two electron orbitals of similar energy, therefore is subject to Jahn–Teller distortion in its octahedral coordination environment—creating a weak point in the hydration shell [15, 17]. As a consequence, Cu was shown to change its coordination environment from outer-sphere to inner-sphere when adsorbed in narrow pores of mordenite (limiting pore diameter 0.26 nm) [15, 17]. As shown by the significantly enhanced surface area normalized adsorption of Cu on SBA-15-4 over SBA-15-6 and SBA-15-8, our data may suggest changes in the adsorption complex geometry due to changes in water properties and steric strain of pore confinement. Our data agrees with previous studies showing that the changes in water properties and subsequent tendency for cations to form inner-sphere complexes preferentially enrich trace elements in nanopores [48, 49]. Wang et al. demonstrated a nearly 10-fold increase in the surface area normalized adsorption of both zinc (Zn2+) and arsenate (AsO43−) on nano-porous alumina compared to alumina particles. Wang et al. attributed the observed increase in adsorption to the increase in the surface charge density inside nano-pores, and the impact of a larger proportion of structured water on ion hydration [2, 48, 50]. Furthermore, another study of uranium U6+ adsorption and desorption on mesoporous silica (MCM-41), demonstrated the formation of polymeric species—and eventual precipitation—inside the pores . It is possible that the surface area normalized adsorption of Cu is enhanced in small mesopores (4 nm) due to Cu losing it hydration shell thus increasing its reactivity towards dimerization and surface adsorption.
Effect of nano-scale confinement on adsorption kinetics
As seen in Fig. 5, the pseudo-first-order kinetic rates are inversely proportional to pore diameter; as the pore diameter decreases, the kinetic rate increases. Previous studies have summarized the dependence of surface tension , density , and dielectric constant  of water. Those parameters were approximated from the publications and added to Fig. 5 to compare to our data. As seen from Fig. 5, the changes in density, surface tension, and dielectric constant of water have a negative correlation with the adsorption kinetics quantified in our study. From these trends, we have concluded that the rate of Cu adsorption could be related to the decrease in the surface tension, density, and dielectric constant of water. These changes in water properties could increase the propensity of Cu to lose its hydration sphere and from inner-sphere complexes with the surface. We believe it is reasonable that these changes in the water properties will impact the rate of adsorption of Cu; as the pore decreases in size, a decrease in surface tension and density would allow more rapid flow inside the pores; a decrease in the dielectric constant would lead to a decrease in the hydration energy of the Cu atom, thus allowing for more rapid adsorption on the surface.
External mass transfer of adsorbate from the bulk solution to the adsorbent surface;
Adsorbate diffusion from external surface into the adsorbent pores;
Adsorption of adsorbate at the surface reactive sites.
Conclusions and future work
This experimental study presents a systematic approach to quantify the effects of nano-scale confinement on metal adsorption. While nano-scale confinement effects have been observed in mesoporous systems, this is the first, to our knowledge, study quantifying nano-scale confinement effects on the adsorption of Cu on mesoporous silica. Through an analysis of the surface area normalized adsorption isotherms and adsorption kinetics of Cu on SBA-15-8, SBA-15-6, ad SBA-15-4, we concluded that nano-scale confinement enhances both the adsorption maximum, and Cu adsorption reaction rate. Evidence of this is shown in the significant increase in the surface area normalized adsorption maximum of Cu on SBA-15-4 compared to both SBA-15-6 and SBA-15-8 across all isotherm models. Further, the pseudo-first-order reaction rate constant increased with decreasing pore size. The intraparticle diffusion model was applied, and it illustrates that external mass transfer diffusion constant increases with decreasing pore size, and we postulate that this rapid film diffusion in 4 nm pores was responsible for the observed increase in reaction rate. Future work should address molecular-scale speciation of Cu associated with mesoporous silica surfaces, using spectroscopic approaches.
We believe this study will aid in the understanding of the impacts of cation adsorption in geologically relevant mesopores. This will increase our ability to anticipate cation fate and transport in shales and tight rocks. Further studies are needed to assess the metal coordination environment as a function of pore size, and correlate any changes in coordination number or bond angles or distances to the observed changes in macroscopic adsorption behavior.
AGI led project development, AGI and AWK designed experimental program and analyzed data. ABT assisted with data collection. All authors, contributed to writing the manuscript. All authors read and approved the final manuscript.
The authors would like to thank Eric Coker for collecting BET on mesoporous silica samples. This work was supported by the US Department of Energy, Office of Science, Office of Basic Energy Sciences, Chemical Sciences, Geosciences and Biosciences Division. Sandia National Laboratories is a multimission laboratory managed and operated by National Technology and Engineering Solutions of Sandia, LLC., a wholly owned subsidiary of Honeywell International, Inc., for the U.S. Department of Energy’s National Nuclear Security Administration under contract DE-NA-0003525.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.
- Weber WJ, Huang WL (1996) A distributed reactivity model for sorption by soils and sediments. 4. Intraparticle heterogeneity and phase-distribution relationships under nonequilibrium conditions—response. Environ Sci Technol 30(10):3130–3131View ArticleGoogle Scholar
- Wang YF et al (2003) Surface chemistry of mesoporous materials: effect of nanopore confinement. Struct Prop Relationsh Oxide Surf Interfaces II 751:121–125Google Scholar
- Ilgen AG et al (2017) Shales at all scales: exploring coupled processes in mudrocks. Earth Sci Rev 166:132–152View ArticleGoogle Scholar
- Sing KSW et al (1985) Reporting physisorption data for gas solid systems with special reference to the determination of surface-area and porosity (Recommendations 1984). Pure Appl Chem 57(4):603–619View ArticleGoogle Scholar
- Logar NZ, Kaucic V (2006) Nanoporous materials: from catalysis and hydrogen storage to wastewater treatment. Acta Chim Slov 53(2):117–135Google Scholar
- Levinger NE (2002) Water in confinement. Science 298(5599):1722–1723View ArticleGoogle Scholar
- Marti J et al (2006) Molecular dynamics simulation of liquid water confined inside graphite channels: dielectric and dynamical properties. J Phys Chem B 110(47):23987–23994View ArticleGoogle Scholar
- Senapati S, Chandra A (2001) Dielectric constant of water confined in a nanocavity. J Phys Chem B 105(22):5106–5109View ArticleGoogle Scholar
- Takei T et al (2000) Changes in density and surface tension of water in silica pores. Colloid Polym Sci 278(5):475–480View ArticleGoogle Scholar
- Nelson JM et al (2014) Probing the mechanisms of pore size dependent geochemistry: effects of meso-confinement on Zn sorption in mesoporous silica. In: abstracts of papers of the American chemical society, vol 247Google Scholar
- Zimmerman AR et al (2004) Protection of mesopore-adsorbed organic matter from enzymatic degradation. Environ Sci Technol 38(17):4542–4548View ArticleGoogle Scholar
- Kim YH et al (2004) Arsenic removal using mesoporous alumina prepared via a templating method. Environ Sci Technol 38(3):924–931View ArticleGoogle Scholar
- Madden AS, Hochella MF, Luxton TP (2006) Insights for size-dependent reactivity of hematite nanomineral surfaces through Cu2+ sorption. Geochim Cosmochim Acta 70(16):4095–4104View ArticleGoogle Scholar
- Zeng H et al (2009) Nanoscale size effects on uranium(VI) adsorption to hematite. Environ Sci Technol 43(5):1373–1378View ArticleGoogle Scholar
- Ferreira DR et al (2012) An electron paramagnetic resonance spectroscopy investigation of the retention mechanisms of Mn and Cu in the nanopore channels of three zeolite minerals. Clays Clay Miner 60(6):588–598View ArticleGoogle Scholar
- Ferreira DR, Schulthess CP, Giotto MV (2012) An investigation of strong sodium retention mechanisms in nanopore environments using nuclear magnetic resonance spectroscopy. Environ Sci Technol 46(1):300–306View ArticleGoogle Scholar
- Ferreira DR, Schulthess CP, Kabengi NJ (2012) Calorimetric evidence in support of the nanopore inner sphere enhancement theory on cation adsorption. Soil Chem 77:94–99Google Scholar
- Moore JW (1991) Copper, in inorganic contaminants of surface water: research and monitoring priorities. Springer, New YorkView ArticleGoogle Scholar
- Cheah SF, Brown GE, Parks GA (1998) XAFS spectroscopy study of Cu(II) sorption on amorphous SiO2 and gamma-Al2O3: effect of substrate and time on sorption complexes. J Colloid Interface Sci 208(1):110–128View ArticleGoogle Scholar
- Cheah SF, Brown GE, Parks GA (2000) XAFS study of Cu model compounds and Cu2+ sorption products on amorphous SiO2, gamma-Al2O3, and anatase. Am Miner 85(1):118–132View ArticleGoogle Scholar
- Rengaraj S et al (2004) Removal of copper from aqueous solution by aminated and protonated mesoporous aluminas: kinetics and equilibrium. J Colloid Interface Sci 273(1):14–21View ArticleGoogle Scholar
- Chiron N, Guilet R, Deydier E (2003) Adsorption of Cu(II) and Pb(II) onto a grafted silica: isotherms and kinetic models. Water Res 37(13):3079–3086View ArticleGoogle Scholar
- Aguado J et al (2009) Aqueous heavy metals removal by adsorption on amine-functionalized mesoporous silica. J Hazard Mater 163(1):213–221View ArticleGoogle Scholar
- Pinkas J (2005) Chemistry of silicates and alumino silicates. Ceram-Silik 49(4):287–298Google Scholar
- Ojeda ML et al (2003) On comparing BJH and NLDFT pore-size distributions determined from N(2) sorption on SBA-15 substrata. Phys Chem Chem Phys 5(9):1859–1866View ArticleGoogle Scholar
- Ravikovitch PI, Neimark AV (2001) Characterization of micro- and mesoporosity in SBA-15 materials from adsorption data by the NLDFT method. J Phys Chem B 105(29):6817–6823View ArticleGoogle Scholar
- Carrott MMLR et al (2001) Adsorption of nitrogen, neopentane, n-hexane, benzene and methanol for the evaluation of pore sizes in silica grades of MCM-41. Microporous Mesoporous Mater 47(2–3):323–337View ArticleGoogle Scholar
- Ndungu K (2012) Model predictions of copper speciation in coastal water compared to measurements by analytical voltammetry. Environ Sci Technol 46(14):7644–7652View ArticleGoogle Scholar
- Langmuir I (1918) The adsorption of gases on plane surfaces of glass, mica and platinum. J Am Chem Soc 40:1361–1403View ArticleGoogle Scholar
- Elkady MF, El-Aassar MR, Hassan HS (2016) Adsorption profile of basic dye onto novel fabricated carboxylated functionalized co-polymer nanofibers. Polymers 8(5):177View ArticleGoogle Scholar
- Nethaji S, Sivasamy A, Mandal AB (2013) Adsorption isotherms, kinetics and mechanism for the adsorption of cationic and anionic dyes onto carbonaceous particles prepared from Juglans regia shell biomass. Int J Environ Sci Technol 10(2):231–242View ArticleGoogle Scholar
- Smith KS (1999) Metal sorption on mineral surfaces: an overview with examples relating to mineral deposits. In: Plumblee GS, Logsdon MJ (eds) The environmental geochemistry of mineral deposits. Society of Economic Geologists, Inc, Littleton, pp 161–182Google Scholar
- Mahmoud MA (2015) Kinetics and thermodynamics of aluminum oxide nanopowder as adsorbent for Fe(III) from aqueous solution. Beni-Suef Univ J Basic Appl Sci 4(2):142–149View ArticleGoogle Scholar
- Vadivelan V, Kumar KV (2005) Equilibrium, kinetics, mechanism, and process design for the sorption of methylene blue onto rice husk. J Colloid Interface Sci 286(1):90–100View ArticleGoogle Scholar
- Freundlich H (1906) Concerning adsorption in solutions. Zeitschrift Fur Physikalische Chemie-Stochiometrie Und Verwandtschaftslehre 57(4):385–470Google Scholar
- Everett JA (ed) (1998) Adsorption models in adsorption of metals by geomedia. Academic Press, San DiegoGoogle Scholar
- Dabrowski A (2001) Adsorption—from theory to practice. Adv Colloid Interface Sci 93(1–3):135–224View ArticleGoogle Scholar
- Polanyi M (1963) Potential theory of adsorption. Science 141(358):1010View ArticleGoogle Scholar
- Corbett JF (1972) Pseudo first-order kinetics. J Chem Educ 49(10):663View ArticleGoogle Scholar
- Creed J, Brockhoff C, Martin T (1994) EPA method 200.8, revision 5.4. Determination of trace elements in waters and wastes by inductively coupled plasma—mass spectrometry. U.E.P. Agency, KnoxvilleGoogle Scholar
- Pollock RA et al (2011) Size and spatial distribution of micropores in SBA-15 using CM-SANS. Chem Mater 23(17):3828–3840View ArticleGoogle Scholar
- Galarneau A et al (2001) True microporosity and surface area of mesoporous SBA-15 silicas as a function of synthesis temperature. Langmuir 17(26):8328–8335View ArticleGoogle Scholar
- Kruk M et al (2000) Characterization of the porous structure of SBA-15. Chem Mater 12(7):1961–1968View ArticleGoogle Scholar
- Zhuravlev LT (2000) The surface chemistry of amorphous silica. Zhuravlev model. Colloids Surf A Physicochem Eng Aspects 173(1–3):1–38View ArticleGoogle Scholar
- Ide M et al (2013) Quantification of silanol sites for the most common mesoporous ordered silicas and organosilicas: total versus accessible silanols. Phys Chem Chem Phys 15(2):642–650View ArticleGoogle Scholar
- Giret S, Hu Y, Masoumifard N, Boulanger J, Juere E, Kleitz F, Lariviere D (2018) Selective separation and preconcentration of scadium with mesoporous silica. Appl Mater Interfaces 10:448–457View ArticleGoogle Scholar
- Kosmulski M (2009) pH-dependent surface charging and points of zero charge. IV. Update and new approach. J Colloid Interface Sci 337(2):439–448View ArticleGoogle Scholar
- Wang YF et al (2003) Nanogeochemistry: geochemical reactions and mass transfers in nanopores. Geology 31(5):387–390View ArticleGoogle Scholar
- Kalluri RK, Konatham D, Striolo A (2011) Aqueous NaCl solutions within charged carbon-slit pores: partition coefficients and density distributions from molecular dynamics simulations. J Phys Chem C 115(28):13786–13795View ArticleGoogle Scholar
- Wang YF (2014) Nanogeochemistry: nanostructures, emergent properties and their control on geochemical reactions and mass transfers. Chem Geol 378:1–23View ArticleGoogle Scholar
- Singer DM, Guo H, Davis JA (2014) U(VI) and Sr(II) batch sorption and diffusion kinetics into mesoporous silica (MCM-41). Chem Geol 390:152–163View ArticleGoogle Scholar
- Malash GF, El-Khaiary MI (2010) Piecewise linear regression: a statistical method for the analysis of experimental adsorption data by the intraparticle-diffusion models. Chem Eng J 163(3):256–263View ArticleGoogle Scholar
- Wei W et al (2016) Biosorption of Pb(II) from aqueous solution by extracellular polymeric substances extracted from Klebsiella sp. J1: adsorption behavior and mechanism assessment. Sci Rep 6:31575View ArticleGoogle Scholar